Non-equilibrium signal integration in hydrogels
Peter A. Korevaar
*, C. Nadir Kaplan
*, Alison Grinthal
, Reanne M. Rust
& Joanna Aizenberg
Materials that perform complex chemical signal processing are ubiquitous in living systems.
Their synthetic analogs would transform developments in biomedicine, catalysis, and many
other areas. By drawing inspiration from biological signaling dynamics, we show how simple
hydrogels have a previously untapped capacity for non-equilibrium chemical signal
proces-sing and integration. Uproces-sing a common polyacrylic acid hydrogel, with divalent cations and
acid as representative stimuli, we demonstrate the emergence of non-monotonic
osmosis-driven spikes and waves of expansion/contraction, as well as traveling color waves. These
distinct responses emerge from different combinations of rates and sequences of arriving
stimuli. A equilibrium continuum theory we developed quantitatively captures the
non-monotonic osmosis-driven deformation waves and determines the onset of their emergence
in terms of the input parameters. These results suggest that simple hydrogels, already built
into numerous systems, have a much larger sensing space than currently employed.
1John A. Paulson School of Engineering and Applied Sciences, Harvard University, Cambridge, MA 02138, USA.2Institute for Molecules and Materials, Radboud University, Heyendaalseweg 135, 6525 AJ Nijmegen, The Netherlands.3Kavli Institute for Bionano Science and Technology, Harvard University, Cambridge, MA 02138, USA.4Department of Physics, Virginia Polytechnic Institute and State University, Blacksburg, VA 24061, USA.5Wyss Institute for Biologically Inspired Engineering, Harvard University, Cambridge, MA 02138, USA.6Department of Chemistry and Chemical Biology, Harvard University, Cambridge, MA 02138, USA. *email:firstname.lastname@example.org;email@example.com;firstname.lastname@example.org
ydrogels play a central role in a wide range of
, from drug delivery12
materials. Much of the recent
interest has focused on enabling hydrogels to deform rapidly
in-phase with speciﬁc inputs from the environment, such as pH13,14
or chemical concentration18,19
. In living
self-organizing amoebas navigating in
ﬁelds of chemoattractant
, to heartbeats adapting to ionic bursts and spikes21
and genetic material reconﬁguring with changing
—often involves coupling multiple chemical
stimuli arriving at separate times and rates. This non-equilibrium
integration is driven by materials that convert each incoming
stimulus into a long-lived active chemical or mechanical
response, often outlasting the duration of the stimulus and
thereby enabling it to be coupled to a later one. We considered
that even simple hydrogels intrinsically possess these same
mechanistic elements. In this way, hydrogels may potentially act
as complex chemical signal integrators and in turn exhibit a wide
range of previously unexplored transient phenomena and sensing
In current strategies, there is a tight, in-phase feedback between
the hydrogel deformations, diffusion, and reversible chemical
reactions, such as protonation/deprotonation7,13,14
, or complexation/dissociation10,18
. This means that
as soon as the stimulus—e.g. protons, divalent ions or reagents—
has been removed from the environment, the gel returns to its
original state. Then, the gel’s response to a subsequent stimulus is
a new, separate, independent event. However, we hypothesized
that introducing species that complex to the gel with variable,
rather than uniformly fast, association/dissociation rates would
enable common hydrogels to act as couplers of different stimuli
separated across time and space. In particular, a slow dissociation
rate should alter the traditional picture: By remaining complexed
to the gel, a chemical stimulus would create a kinetically stable
state with a characteristic lifetime. In such a case, the gel’s
deformation would be transiently maintained upon removal of
the stimulus from the environment. A second chemical species
introduced later could then compete for binding sites, and trigger
decomplexation of the
ﬁrst chemical species. As a result, the
complexation, diffusion, and gel deformation rates associated
ﬁrst stimulus become interlinked with those of the
sec-ond. In this paper, we show how coupling the dynamics of
otherwise separate stimuli in time and space creates speciﬁc
responses arising from the transient superposition of chemical
species entering and exiting the gel.
We explore this concept with a widely used hydrogel,
poly-acrylic acid (PAA). Our system consists of a thin layer of hydrogel
containing an array of embedded microplates, which enable
real-time visualization of the gel’s deformations at the microscale. The
hybrid hydrogel-microplate conﬁguration25
enabled a class of adaptive materials that catch and release
, switch chemical reactions on and off27
, or control
. Under neutral or basic
conditions, the carboxyl groups (COOH) of the PAA gel exist in a
deprotonated form (COO−
), the gel is swelled, and the embedded
microplates stand upright. Consistent with the traditional use of
PAA gel as a direct pH sensor, exposure to acid protonates the
groups, inducing nearly immediate contraction of the gel
and the associated tilting of the microplates (Fig.
Adding a base rapidly deprotonates the gel and restores the
ori-ginal state. To test our hypothesis, we apply as a
divalent copper ions (Cu2+
), which interacts with COO−
contracts the gel. Cu2+
form a kinetically stable
chelate complex, which has been reported to maintain localized
gel deformation and blue color over months in the absence of
Our results demonstrate how this
blue color, characteristic for COO−
provides a complementary readout mechanism for the complex
kinetic interplay between two stimuli. When acid (H+
deliv-ered as a second stimulus to a system previously exposed to Cu2+
competes for COO−
b, gray box) and displaces
, releasing it into the
ﬂuid phase of the gel and then into the
initially copper-free supernatant. Cu2+
decomplexation will be
dependent on the timescale of acid delivery
with respect to the timescales of Cu2+
diffusion and hydrogel
deformation leads to the emergence of a variety of competing
non-equilibrium dynamics (Fig.
, expanded gray box).
Through experiments, scaling laws and a non-equilibrium
continuum theory that captures the time-dependent coupling of
the two stimuli, we demonstrate how two different, previously
unseen responses emerge. (i) Acid-induced Cu2+
inside the gel triggers transient water inﬂux, driven by the
osmosis caused by the Cu2+
ions released into the
ﬂuid phase of
the gel (dependent on the timescale of acid delivery
). At the
same time, acid itself contracts the gel (with the mechanical
). Counterintuitively, even though both Cu2+
contract the gel upon complexation, the competition
-induced osmosis and acid-induced contraction
produces traveling osmotic swelling waves when
c). (ii) If copper is complexed locally in the hydrogel, acid
in region A to diffuse and recomplex to new COO−
groups in previously unoccupied neighboring regions B (Fig.
At the same time, acid also competes with Cu2+
and displaces it
from these new sites. As a result, traveling color waves appear
ahead of a slow-moving acid front when it progresses more
slowly than Cu2+
Delivering the Cu2+
stimulus to the hydrogel-microplate
sys-tem. Our hydrogel system comprises an array of surface-attached,
slightly pretilted epoxy microplates embedded in a PAA hydrogel
a). The plates are 18 µm tall. The hydrogel has a height of
≈ 10 µm measured from the confocal microscopy z-stack
ima-ging (Supplementary Fig. 1). After deprotonating the PAA
hydrogel by rinsing with a base, the hydrogel is swollen and the
microplates are oriented nearly upright, 9° with the surface
normal (see Methods for details). Upon addition of an aqueous
copper(II)sulfate solution (0.8 M CuSO4
), the hydrogel turns blue,
indicating the formation of COO−
the hydrogel (Fig.
b, c). Concurrently, the hydrogel contracts,
and the embedded microplates tilt toward the substrate. This is
evidenced by a progressive conversion from a rectangular to a
square projection of the microplates in plain-view optical
microscopy images. We note that the presence of the microplates
and the blue color of the gel provide simple visual reporters on,
respectively, (i) the deformation state of the gel, which is
quan-tiﬁed by the microplate tilt angle, and (ii) Cu2+
which is quantiﬁed by the red channel (r-) value in optical
microscopy images (see Methods and Supplementary Fig. 1).
Both the microplate tilting and the blue color are maintained after
is removed from the external solution, even after repeated
rinsing with water, indicating a kinetically stable state that
stores the Cu2+
stimulus upon complexation. The vertical
dif-fusion of Cu2+
into the gel layer happens at a timescale
≈ 10 s, with a diffusion constant of DCu2+
. Thus, we expect the local contraction and coloring
responses upon Cu2+
delivery to occur over a time
layer of a sodium perchlorate electrolyte solution (NaClO4
0.05 M, see Scheme in Fig.
d, Methods and Supplementary
Fig. 2). When a voltage of approx. 1 V (current 0.1 mA) is
applied, the microplates near the positive electrode begin to tilt as
the corresponding region of the hydrogel contracts and turns
blue. The region expands outward in time with a gradient of tilt
angles and color intensity, consistent with Cu2+
from the electrode through the electrolyte and binding to the
e and Supplementary Movie 1). The slight initial
pretilting of the microplates in one orientation results in a
uniform tilting direction upon Cu2+
-complexation. As we
noticed a variability in the degree of gel contraction depending
on the direction of electrochemical Cu2+
delivery, all experiments
were performed such that the pretilted plates were oriented
towards the Cu2+
source, as schematically represented in Fig.
Both the tilted state and blue color are maintained after Cu2+
removed from the external solution by rinsing the substrate with
water. Only a slow release of Cu2+
occurs at the edge of the
-contracted region (Fig.
Osmotic pulses and waves selective to rapid Cu2+
kinetically stable complexation creates a unique condition where
is present inside the gel and absent from the external
environment. Hence, rapid dissociation of Cu2+
protona-tion of the carboxylates must yield a transient osmotic pressure
within the gel (Fig.
a): If the release rate of Cu2+
is fast enough
to induce water inﬂux, this triggers an osmotic imbalance across
the gel−supernatant solution interface. Satisfying this condition
requires the relaxation time of the hydrogel deformation
be smaller than the diffusion timescale of Cu2+
ϵ Δh=H is the ratio of the change
ﬁlm thickness Δh over its equilibrium thickness H, L is the
horizontal length scale, and U(0)
is the inlet speed of the acid).
Acid rate > Cu2+ diffusion rate:
no color wave H+ < ⊥ : osmotic swelling wave H+ > ⊥ : no osmotic swelling
Acid rate < Cu2+ diffusion rate:
color wave C C
bHydrogel Microplate Very slow dissociation C C CO O O O O O O O O O O O O O O O O– O– O– O– O– O– O– O O – O – O – O – O – O – O – O C C C C C C C C C C C
Competition: Acid-induced Cu2+ release time H+
vs. mechanical relaxation time ⊥
Competition: Acid front progression rate vs. Cu2+ diffusion rate Acid front Water influx Acid front Cu2+ efflux
dC C C C C Released Cu2+
Localized osmotic swelling
Gel S upernatant
cC C C C C C O O O O O O O O O O O O OH OH HO HO C Emergent response mechanisms A H+ H+ A B B ⊥ H+ H+ H+ H+ O O O H+ H+ Cu2+ Cu2+ Cu2+ O O– O– O– – O – O – O OH HO
Fig. 1 Non-equilibrium coupling of stimuli across time. a Traditionally, a responsive polyacrylic acid (PAA) hydrogel contracts and swells directly in-phase with the presence or absence of an acid stimulus (yellow). Here, hydrogel contraction tilts an array of embedded microplates (gray).b In contrast to this rapid reversibility, divalent cations (Cu2+, blue) contract the PAA gel by forming a kinetically stable complex with two carboxylate (COO−) groups, remaining in the gel after removal of Cu2+from the environment. A subsequent acid stimulus then competes for COO−groups and triggers dissociation of the Cu2+on a timescale determined by its delivery rate (τH+). The ensuing dynamics of diffusion, complexation, and mechanical deformations in the
presence of the entering and exiting stimuli can lead to scenarios depicted in c-d:c Competition between transient water inﬂux, induced by released Cu2+, and the mechanical relaxation time of the gel (τ⊥) creates traveling osmotic swelling waves reporting the speed of an oncoming acid front whenτH+<τ⊥;
Then, a sufﬁciently low acid-induced Cu2+
, is expected to produce an unusual transient
gel swelling that would be selective only to fast onset-rates of the
As an initial test of this scaling prediction, a concentrated acid
solution (1 M HCl) was added to a hydrogel-microplate substrate
containing complexed Cu2+
. Directly after this delivery of a
arriving’ acid stimulus, a rapid dissociation of Cu2+
as indicated by the loss of blue color within
≈ 2 s (Fig.
and Supplementary Movie 2). Concurrent with this color
transition, the initially tilted microplates brieﬂy stood upright at
the onset of the acid stimulus, conﬁrming that the system reports
the fast acid
ﬂow with a transient swelling of the hydrogel when
, and then tilted back toward the substrate over
10 s. Corroborating that this unique transient swelling is indeed
driven by an osmotic imbalance induced by Cu2+
show that the inclusion of CuSO4
(0.8 M) in the HCl solution—to
reduce its hypotonic character—suppresses the swelling pulse
(Supplementary Fig. 3).
To assess the selectivity of the swelling response for fast Cu2+
release, the same amount of acid was added slowly via a series of
progressively concentrated HCl solutions, from 0.01 to 1 M. As
shown in Fig.
c, e, Cu2+
dissociates from the hydrogel during the
addition step of 0.05 M HCl, over
≈ 20 s. Since in this case the
generation of free Cu2+
inside the gel is slower than its diffusion
out of the gel (i.e.
≈ 10 s), the accumulation of free
in the gel is insufﬁcient to drive the osmotic swelling. As a
result, the gel is observed to remain in its contracted state with the
microstructures titled to the substrate, and simply changes color
as protonation induces the release of Cu2+
. We note that when
) is used as an alternative complexing agent to
contract the PAA hydrogel, Ca2+
release upon rapid addition of
acid induces a transient swelling response as well (Supplementary
Fig. 4), suggesting a general applicability of our approach.
The transient osmotic pressure due to rapid Cu2+
can also take the form of traveling swelling waves that are
sensitive to the progression rate and direction of an acid front
spreading across the substrate. As schematically shown in Fig.
an acid stimulus with a controllable progression rate can be
initiated by delivering a drop of acid under one edge of a
glass cover (Methods and Supplementary Fig. 5). Cu2+
decom-plexation at the acid front is indicated by a blue-to-colorless
transition that progresses from left to right (Fig.
b, c), and occurs
over a length scale of L
≈ 100 µm, consistent with free diffusion
within the stimulus front (D
≈ 10 s
≈ 10 s (see Supplementary Information). To meet the110 130 150 5 15 25 35 0 5 10 15 r-value (–) r-value (–)
Microplate tilt angle (°) Microplate tilt angle (°)
Add Cu2+ Remove stimulus from environment
Rinsed with water Pure water Cu2+ delivery + –
d130 150 170 5 15 25 35 0 100 200 x (μm) t′ = 1 h in water t′ = 0 t′ = 0 65 s 130 s
ct = 0 t = 1 h t = 0 t = 1 h
eCu2+ Cu2+ Cu2+
≈ 10 s—the requirement for observing
a transient swelling response as discussed above, where
—the acid progression speed must be vC
> 10 µm s−1
Consistent with this prediction, a wave of weakly up-and-down
moving microplates is experimentally observed to travel at the
front of an acid stimulus moving with a minimum rate of vC
8.6 µm s−1
c and Supplementary Movie 3). A slower
progression yields no swelling pulse at the stimulus front
(Supplementary Fig. 6), as exempliﬁed by the results in Fig.
acquired at vC
= 0.76 µm s−1
. In contrast, fast progression (vC
95 µm s−1
) yields a high-amplitude traveling pulse (Fig.
pressure that is required to establish a swelling wave spreading
≈ 100 µm within τH+
≈ 10 s determines the poroelastic
diffusion constant of water inside the hydrogel, given by Dwater
hydraulic permeability of the hydrogel and
Pa s is
the dynamic viscosity of water. The required pressure
1−10 MPa; a pressure that can be generated upon osmosis as the
concentration of Cu2+
ions is estimated to be 2.9 M
(Supple-mentary Fig. 7 and Supple(Supple-mentary Information), implying a
maximum osmotic pressure of ~7 MPa (posm
note that the orientation of the microplates with respect to the
acid stimulus progression does not have a major effect on the
swelling response of the hydrogel.
To further assess the timescales and forces involved in the
unique transient swelling responses and traveling waves that arise
upon coupling of successive Cu2+
and acid stimuli, we developed
a continuum theory that gives the time-dependent height proﬁle
of a thin hydrogel sheet, based on time- and position-dependent
descriptions of (i) Cu2+
and acid present in the supernatant
in the hydrogel interior
ﬂuid, and complexed to PAA; (ii) the
osmotic and contractile forces exerted on the gel due to free and
and acid in the gel, and (iii) the mechanical
deformation of the gel (see Supplementary Discussion).
Simula-tions based on parameter values, which match experimentally
assessed time- and pressure-scales, quantitatively reproduce the
experimental vertical deformation waves of the hydrogel, as
derived from the experimentally observed microplate tilting
e, Supplementary Figs. 8 and 9, and Supplementary
Movies 4–6). The transient osmotic vertical ﬂow for thin ﬁlm
domains is given by Supplementary Eq. 14 and holds at the
leading order O(δ0
δ is the aspect ratio of the thin ﬁlm;
ϵ and δ are very small. The mobility coefﬁcient in
Supplementary Eq. 14 scales with
and is not a free parameter.
ﬂow term quantitatively reproduces the
osmosis-induced traveling waves (Fig.
, Supplementary Movies 4–6).
Thereby, our theory shows that,
ﬁrst, species released within the
hydrogel induce transient osmosis; second, this enables unique
signaling routines that selectively report input stimuli occurring
at fast rates; and, third, swelling pulses are displayed at timescales
that cannot be established by solely breaking crosslinks in the
hydrogel.10 15 20 25 –2 0 2 4 6 8 10 12 14 100 125 150 175 Time (s)
Microplate tilt angle (°)
r-value (–) 1 M directly 100 125 150 175 10 15 20 25 0 50 100 150 t′ = 0 s 1 s 2 s 4 s Addition of 1 M HCl (Regime H+ < ⊥ ) Addition of 0.05 M HCl (Regime H+ > ⊥ ) 0 s Time (s) 0.01 M 0.05 M0.1 M 0.5 M1 M Downstream stimulus: HCl additions 1 M HCl Start 1 M HCl Start Pulse Fast release of Cu2+
e1 s 2 s 3 s 5 s 8 s 11 s 18 s No pulse Slow release of Cu2+ C C C C C C C O OH O H O O O O– O O O O O– O– – O – O – O C C O O O H O H C Osmotic swelling pulse
Ion exchange in contracted state
Fast Slow –Cu2+
aFinal contracted state Cu2+ stored H+ < ⊥ H+ > ⊥ Cu2+ Cu 2+ Cu2+ Cu2+ H+ H + H+ H+
Fig. 3 Cu2+ions generate a transient osmotic swelling pulse upon rapid release by an acid stimulus. a Schematic presentation of the mechanism, showing how acid delivered after Cu2+has been removed from the external environment of the hydrogel protonates carboxylate groups and thereby releases the complexed Cu2+. Fast release would generate an osmotic swelling pulse (top) before acid contracts the hydrogel again, while slow addition of acid should lead to a slow Cu2+release without transient swelling (bottom).b Experimental demonstration of the fast Cu2+release (regimeτH+<τ⊥), triggered by direct addition of concentrated 1 M HCl, which results in rapid disappearance of the blue color and transient reorientation of the microplates to an upright position. The dotted outlines indicate the change of the cross-sectional view of a single plate from nearly square (in the tilted state) to rectangular (in the upright state), and back to nearly square.c Stepwise addition of acid leads to a slow release of Cu2+, such that the gel remains contracted without transient swelling (regimeτH+>τ⊥). Scale bar: 25μm. d, e Time-dependent microplate tilt angle and r value (acid stimulus added at t =
Traveling color waves reporting slow acid fronts. Copper ions
released by acid from the hydrogel into an otherwise Cu2+
medium not only enable short-term osmotic pressure in the gel,
but also give rise to localized patterns of recomplexation as the
ions diffuse with the moving acid front. While
swelling waves require a rapidly moving acid front to trigger a
rapid release of Cu2+
inside the gel, recomplexation of Cu2+
should in contrast require the acid front to be moving slowly
enough for the diffusing Cu2+
ions to be able to compete with the
oncoming protons for new binding sites. Assuming a graded acid
concentration at the front, Cu2+
comigrating with the front will
potentially have a time window to recomplex to the gel in the
presence of a low acid concentration, before saturating acid
overtakes the recomplexed Cu2+
and releases it again. Consistent
with this possibility,
ﬂowing a solution containing 1 M HCl and
0.8 M CuSO4
with a slow progression rate along a substrate with a
deprotonated PAA hydrogel yields a transient band of Cu2+
complexation at the solution front (vC
= 3 µm s−1
Supplemen-tary Fig. 10). For a system that is exposed
ﬁrst to Cu2+
subsequently to progressing acid, initial release of Cu2+
by acid at0 s 75 s 115 s 155 s 195 s 250 s 0 s 4 s 6 s 8 s 10 s 22 s 0 s 1 s 2 s 4 s 6 s 16 s C= 0.76 μm s–1 (H+ > ⊥) C= 1.1 μm s–1 C= 8.5 μm s–1 C= 95 μm s–1 C≥ 95 μm s–1 (H+ < ⊥) C= 8.6 μm s–1 (H+≈ ⊥)
dStimulus: infuse HCl (1 M) Glass cover
a0 s 250 s 0 s 22 s 0 s 16 s Relativ e gel height (–) x (μm) Wave Pulse x (μm) x (μm)
eRelativ e gel height (–) 0.9 1 1.1 0 50 100 150 0 50 100 150 0 50 100 150
Progressing acid front
Starting hydrogel 26 s 51 s 77 s 3 s 7 s 10 s 0.3 s 0.6 s 1 s x (μm) x (μm) x (μm) 100 120 140 r -value (–) H+ H+ 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0.95 0.9 0 50 100 150 0 50 100 150 0 50 100 150
Fig. 4 Traveling swelling waves that are sensitive to the acid progression rate. a Schematic of the experimental design: HCl (1 M) is added from the left side of a Cu2+-contracted substrate covered with a thin waterﬁlm and a glass cover (see Methods). b–d (Top) Micrographs showing the progression of the acid stimulus at various rates, indicated by a blue-to-colorless transition. (Bottom) The height of the diagrams represents the evolution of the relative hydrogel height in time and space derived from the microplate tilt angle as described in Methods (Supplementary Fig. 1), along the white dashed line for the six micrographs from top to bottom; and the color of the diagrams represents the Cu2+release as characterized by the blue-to-colorless transition:b No swelling pulse is observed for the acid stimulus that travels from left to right over 190μm in 250 s (vC= 0.76 μm s−1);c, d Faster progression of the acid
within 22 s (cvC= 8.6 µm s−1) and within 2 s (dvC≥ 95 µm s−1) generates swelling/contraction waves that travel at the acid front. Scale bar: 25µm. e The
results of our continuum theory show that traveling swelling/contraction waves are only obtained atvC≥ 8.5 µm s−1for this set of experimental
a region A, followed by diffusion of Cu2+
super-natant solution and recomplexation to the gel at a region B, can
result in a transient band of Cu2+
complexation. This must only
happen when acid migration from A to B is slower than the
diffusion of Cu2+
and its subsequent recomplexation at B: Lx
, where Lx
≈ 100 μm is the distance between
A and B, and D(a)
is the diffusivity in the supernatant solution.
To test this idea, we electrochemically delivered Cu2+
one half of a gel/microplate system, so that Cu2+
is stored on one
side while the other remains copper-free (blue and white sides in
a, respectively). Acid is then
ﬂowed such that the front
progresses over both halves in parallel (Fig.
a, yellow). This
conﬁguration potentially allows some of the released Cu2+
front to diffuse to and recomplex on the copper-free side, subject
Fast (C = 225 μm s
–1) | acid rate > Cu2+
diffusion rate: no color wave
t = 0 s 240 s 330 s t = 0 s 2 s 13 s
Locally delivered first
chemical stimulus (Cu2+) Directional addition of the
second chemical stimulus (droplet of 1 M HCl)
Fast or slow progression of acid along substrate
Slow (C = 1 μm s
–1) | acid rate < Cu2+
diffusion rate: color wave
Cu 2+ complexed No Cu 2+ Cu 2+ complexed No Cu 2+
f5 15 25 35 110 130 150 170 5 15 25 35 –5 0 5 10 110 130 150 170 –5 0 5 10
Microplate tilt angle
Microplate tilt angle
(°) Time (s) Time (s) 5 15 25 35 110 130 150 170 5 15 25 35 80 180 280 380 110 130 150 170 80 180 280 380 Blue wave Microplate tilt ang
r-value (–) r-value (–)
r-value (–) Microplate tilt angle (°)
Time (s) Time (s) C O O O O O O O O O O H OH OH H O O H H O H O H O O O– O O O– – O O O O O O O O– – O O– – O O O O– – O – O C C C C C C C C C C C C O O O H O H OH HO HO HO C C O O C C C C C C C C C Osmotic pulse Blue wave
dOsmotic pulse – + Cu2+ H+ H+ Cu2+ Cu2+ Cu2+ Cu2+
to the acid-dependent competition and time window. Our
experimental results at different progression speeds indeed
indicate the ability of this mechanism to produce a distinctive
slow-rate-sensitive response: a slow acid progression speed (vC
1 µm s−1
) generates a wave of blue color that travels with the acid
front through the initially copper-free side (Fig.
b, d, f and
Supplementary Movie 7), featuring the regime where the acid
progression is slower than the Cu2+
diffusion. This response was
further observed with an intermediate rate of vC
= 3 µm s−1
(Supplementary Fig. 11), and also with a hydrogel without
embedded microplates (Supplementary Fig. 12). The inequality
only holds when vC
< 5 µm s−1
= 10 s. Indeed, at fast
progres-sion rates (vC
= 225 µm s−1
c, e, g), no blue color was
observed on the copper-free side (acid progression rate > Cu2+
diffusion rate). Instead, a wave of osmotic pressure was generated
on the copper-storing side, with the associated transient upright
movement of the microplates, as discussed above.
Our results provide a potentially transformative approach to
chemical signal processing and, more generally, suggest that
simple hydrogels have a much larger sensing space than is
cur-rently made use of. By integrating the
complexation-transport-deformation dynamics induced in the gel by two chemical stimuli
that occur separately in time and space, we show that a common
hydrogel—traditionally used for direct stimulus tracking through
nearly in-phase response to an applied stimulus—can produce
previously unseen complexity. This is demonstrated by
time-sensitive, nonmonotonic osmotic effects accompanied by spikes
and waves of gel expansion and contraction, as well as traveling
color waves of patterned migration and recomplexation. Our
non-equilibrium continuum theory captures how the diverse
responses depend on the coupling of diffusion,
complexa-tion, and hydrogel deformation as successive chemical stimuli
enter and exit the gel. The theory allows the parameter windows
to be predicted for a range of phenomena based on the relative
timescales involved in signal coupling. Combined with an
extensive experimental and scaling analysis, the model provides
insight into the competing processes underlying the response
mechanisms and emergent behaviors. As exemplary cases, our
theory reveals how traveling osmotic swelling waves can emerge
in response to the rapid onset of a stimulus that would normally
—on its own—contract the gel, if the timescale of acid
propa-gation is smaller than the mechanical relaxation time of the
hydrogel. The theory further implies that, when two H+
approach from opposite directions, the accompanying swelling
fronts would annihilate each other upon collision. This is because
no available bidendate complexation sites would be left ahead of
each front to be decomplexed and create osmotic imbalance.
Further scaling laws elucidate how a slowly moving acid gradient
can induce sequences of migration and recomplexation highly
sensitive to the interdependent dynamics of the released and
In conclusion, the framework presented here shows how a
hydrogel can be used without specialized modiﬁcations to
per-form complex chemical sensing tasks not previously achieved
with electronics-free systems. The exemplary responses we
demonstrate likely represent only a small sample of the dynamic
phenomena that may emerge. Based on simple, reversible
chemistry and trivial hydrogel composition and geometry, our
scaling analyses and the theoretical model elucidate distinct
outputs able to discriminate among many possible combinations
and permutations of rates, times, sequences, and conﬁgurations
of multiple arriving stimuli. These concepts are potentially
applicable to a wide range of hydrogels, stimuli and
non-equilibrium molecular systems beyond the ions, acid, and PAA
gel used in this study.31–39
The non-equilibrium concepts and
theory can be further applied to readout mechanisms beyond the
microplates used in this study, such as via microparticles
dis-persed within the gel or via focussing and defocussing of light
beams by the gel. Additionally, the concept of rate-selective
recomplexation waves—exempliﬁed by the blue color waves in
our system—can be expanded by selecting alternative pairs of
complexing agents (such as Ca2+
), potentially in
ﬂuorescent or other indicators. In particular, the
non-equilibrium mechanisms revealed in this study may enable
micron-scale synthetic soft actuators, analogous to the way Ca2+
-based biochemical reaction-transport pathways power the motion
of some single-celled organisms, such as D. discoideum40
. Beyond reporting the gel’s dynamics,
microstructures embedded in the gel can themselves introduce
feedback to the complexation-transport-deformation coupling42
potentially opening another realm of non-equilibrium sensing.
Further developing these capacities may bring about new
possi-bilities for integrating complex chemical sensing and
transduc-tion, using simple soft materials, into areas such as soft robotics,
catalytic materials, and agricultural and biomedical diagnostics.
Chemicals and materials. Polydimethylsiloxane (PDMS, Dow-Sylgard 184) was purchased from Dow Corning Corporation (Midland, MI, USA). Epoxy resin OG178 was purchased from Epoxy Technology (Billerica, MA, USA). Glycidyl methacrylate, acrylic acid, sodium acrylate, 2,2′-azobis(2-methylpropionamidine) dihydrochloride, N-N′-methylenebisacrylamide, 1-butanol, ethylene glycol, copper (II)sulfate, sodium perchlorate, ethylenediaminetetraacetic acid, potassium hydroxide and hydrochloric acid were purchased from Sigma Aldrich. Irgacure 819 was purchased from BASF Corporation, Lumiprobe BDP FL NHS ester from Lumiprobe Corporation (Hallandale Beach, FL, USA), calcium chloride from J.T. Baker and copper(II)chloride from Fluorochem. All compounds and materials were used as received.
Fabrication of hydrogel-embedded microplate substrates. To prepare the epoxy microplate substrates,ﬁrst a PDMS negative mold was obtained by curing a 10:1 wt./wt. mixture of base resin and hardener onto a silicon master with the micro-plates positioned in a staggered array, with a height of 18 µm, a width of 10 µm, a thickness of 2 µm and a spacing of 5 µm in both x and y directions. The silicon master was fabricated via the Bosch process and functionalized with (trideca ﬂuoro-1,1,2,2-tetrahydrooctyl)trichlorosilane in a desiccator under vacuum at room temperature for at least 24 h, in order to facilitate demolding of the PDMS. The PDMS prepolymer mixture was mixed for 1 min, degassed under vacuum at room temperature, poured over the silicon master in a petri dish, put under vacuum at room temperature to remove bubbles, and then cured at 70 °C. After 2 h, the PDMS molds were cooled and peeled off from the silicon mold. To prepare an epoxy microplate substrate, 35 µL of a 9:1 (wt./wt.) prepolymer mixture of the OG178 epoxy resin and glycidyl methacrylate was added to the PDMS mold and covered with a glass slide (16 × 16 mm2, pretreated in O2-plasma for 2 min). UV curing was performed under a UV lamp (100 W, Blak-Ray with a 365 nm band-passﬁlter, approx. 10 mW cm−2at 365 nm) for 30 min. The microplate substrate was then obtained by carefully removing the glass slide from the PDMS mold.
In order to embed the microplate structures in the hydrogel, 3 µL of a hydrogel precursor solution was added to the substrate. The hydrogel precursor solution was prepared by combining 400 µL of acrylic acid with 20 mg N-N
′-methylenebisacrylamide crosslinker in 1 mL of a 1:1 v/v mixture of ethylene glycol and 1-butanol. To introduce the Irgacure 819 photoinitiator, 10 µL of a 25 mg mL−1solution in 1-butanol was added to 90 µL of the aforementioned solution to obtain the hydrogel precursor solution. After applying the hydrogel precursor solution to the microplate substrate, it was immediately covered with a thin glass cover slide (cleaned with isopropanol) and the hydrogel was subsequently cured for 5 min under UV, similarly to the epoxy curing. After curing, the hydrogel-microplate substrate was immersed in deionized water to allow the glass cover slide to detach and to exchange the ethylene glycol/1-butanol mixture in the hydrogel for water.
To assess the embedding of the microplates in the hydrogel, the hydrogel was dyed by combining a solution of Lumiprobe BDP FL NHS ester (2.5 mg mL−1) in a 1:1 v/v 1-butanol/ethylene glycol mixture with an equal volume of a double concentrated hydrogel precursor solution (see above). Next, the obtained solution was applied to the microstructures and cured as described above. The dyed hydrogel-microplate substrates were then analyzed by confocal microscopy (λex=
To prepare a hydrogel substrate with no microplates embedded,ﬁrst an epoxy substrate was prepared by photo curing a Norland 68 epoxy resin sandwiched between aﬂat PDMS support layer and a glass cover (prepared as described above, total exposure time under UV 10 min). Subsequently, 40 µL of a hydrogel precursor (113 mg mL−1sodium acrylate, 11 mg mL−1N-N′-methylenebisacrylamide and 7.5 mg mL−12,2′-azobis(2-methylpropionamidine) dihydrochloride photoinitiator in water) was applied, and covered with a glass slide of 18 × 18 mm2. Subsequently, the hydrogel was cured under UV (366 nm, 4 min) and the substrate was immersed in water to detach the glass cover. Then, the substrate was vertically immersed for 2 min in an aqueous CuCl2(0.8 M) solution, such that one half of the hydrogel was
complexed to Cu2+as evidenced by the appearance of blue color. The results in Supplementary Fig. 12 were acquired in analogy to the methodology applied for Fig.5; the images were acquired on a Leica DM 2500 microscope equipped with a Leica DFC 7000T camera.
Assessing complexation of Cu2+and tilting of microplates. All optical microscopy images were acquired with an Olympus IX71 darkﬁeld inverted microscope equipped with a QImaging Retiga 2000R camera unless stated other-wise. All colored images were acquired with similar white balance settings and light intensity. Confocal microscopy was performed using a ZEISS LSM 700 microscope. SEM images were acquired on a JEOL JSM 639OLV scanning electron microscope, and the sample was sputter-coated with Au/Pd for imaging.
To quantify the tilting of the microplates, the microplate tilt angle was determined from the microplates’ projection in optical microscopy images. The projection of the microplates was measured in the images and, based on the ratio of this projection to the distance between n rows of microplates in the same image, which equals (n– 1) × 7 μm, converted to the real dimensions p in μm. Based on the height of the microplates h= 18 μm and the thickness t = 2 μm, the microplate tilt angleα was determined as α = 90− acos((p − t)/h) (see Supplementary Fig. 1c). It is assumed that the plates do not curve upon actuation but maintain their straight form and only hinge at the connection to the substrate (see Supplementary Fig. 1b). The relative gel height was derived via cos(α)/cos(αgel completely swelled).
The color proﬁles were acquired using ImageJ 1.50b software. To avoid the proﬁles being disturbed by the contours of the microplates, the images were blurred (Gaussian blur; Sigma radius 50) prior to acquiring the r value (red channel RGB value).
Absorption spectra were acquired on a Beckman Coulter DU 720 UV/Vis spectrometer, in a polymethyl methacrylate (PMMA) cuvette (optical path length 1 cm) at room temperature, and the background was acquired on a PMMA cuvette with water.
Complexation of Cu2+in the hydrogel. Prior to the contraction of the hydrogel via Cu2+complexation, the hydrogel-microplate substrate was sequentially rinsed with hydrochloric acid (HCl 1 M, 4× the same solution of 2 mL), water (5×), potassium hydroxide (KOH in a concentration of 0.1 M, 4× the same solution of 2 mL, repeated with a fresh solution of 2 mL), and water (5×). Thereafter, excess water was removed from the substrate with a tissue. For Fig.2b, a thin layer of 50 µL water was applied to the substrate, and subsequently 10 µL CuSO40.8 M was
added. To assess the storage of Cu2+upon complexation to the hydrogel, the substrate was rinsed with water (4×).
Electrochemical delivery of Cu2+. Cu2+ions were delivered to the hydrogel-microplate substrate by mounting a copper wire (diameter approx. 100μm) as a positive electrode and a copper mesh (hole and wire diameter approx. 100μm) as a negative electrode on top of the substrate with scotch tape, with a distance between the (+) and (–) electrodes of approx. 3 mm, as schematically represented in Fig.2d. The scotch tape was applied such that it did not allow a short-circuit between the electrodes. One hundred microliters sodium perchlorate (NaClO4) in water
(0.05 M) was added as an electrolyte solution, forming a thin electrolyte layer that ensured contact with both the (+) and (–) electrodes. The electrodes were con-nected via crocodile clips to a Keithley 2450 Sourcemeter power supply, and the current was set at 0.1 mA, resulting in a voltage of approx. 1 V.
Swelling and contraction pulses. To prepare the hydrogel for Cu2+ complexa-tion, the hydrogel was rinsed with hydrochloric acid (HCl 1 M, 4× the same solution of 2 mL), water (5×), potassium hydroxide (KOH 0.1 M, 4× the same solution of 2 mL, repeated with a fresh solution of 2 mL), and water (5×). Subse-quently, excess water was removed from the substrate with a tissue, 50 µL of a 0.8 M CuSO4solution was added, excess Cu2+was removed by rinsing the substrate
with water and excess water was removed with a tissue. To obtain the swelling/ contraction pulse (Fig.3b), 1 mL 1 M HCl was added. The stepwise addition of HCl solutions with increasing concentrations (Fig.3c) was performed by adding volumes of 1 mL, with removal of excess HCl solution from the substrate prior to each subsequent addition.
Controlled progression of acid stimulus. Cu2+wasﬁrst complexed to the hydrogel as described above (swelling and contraction pulses). The substrate was then dried with a tissue, 4μL water was applied, and the substrate was covered with a 10 × 16 mm2glass cover of 1 mm thickness. To initiate the HCl stimulus, a
droplet of 30 µL 1 M HCl was added at the edge of the glass cover as schema-tically shown in Fig.4a. The color transition progression speed vCin µm s−1was
determined via the time it took the blue-to-colorless front to progress from left to right over theﬁeld of view (190 µm). Small-magniﬁcation optical microscopy images in Supplementary Fig. 5 reveal a fast progression of the HCl front over theﬁrst few millimeters, whereas further away from the edge of the glass cover the progression of the HCl front slows down, enabling variation of vCfor
dif-ferent experiments shown in Fig.4and Supplementary Fig. 6. Alternatively, a larger amount of water under the glass cover can be used to slow down the progression.
Spatial patterning of pulses and traveling waves. To obtain a localized Cu2+ complexation (Fig.5), Cu2+was electrochemically delivered via the same proce-dure as described above (electrochemical delivery of Cu2+). Here, the experiments started with a substrate that was rinsed with hydrochloric acid (HCl 1 M, 4× the same solution of 2 mL), water (5×), potassium hydroxide (KOH 0.05 M, 4× the same solution of 2 mL, repeated with a fresh solution of 2 mL), and water (5×). Subsequently, the electrodes were removed, and the substrate was rinsed with water, dried with a tissue, and covered with 4 µL water and a glass cover (10 × 16 mm2, 1 mm thick). Similarly to the procedure described above (Controlled progression of acid stimulus), a droplet of 30 µL 1 M HCl was added at the edge of the glass cover to initiate the Cu2+release, as schematically shown in Fig.5a.
Determining the concentration of Cu2+complexed to gel. The concentration of Cu2+complexed to the COO−groups in the hydrogel was determined upon extraction of Cu2+from the hydrogel with an ethylenediethylaminetetraacetate (EDTA) solution, as shown in Supplementary Fig. 7. By comparing the optical density of the extract solutions to a calibration line (based on absorption spectra of aqueous EDTA solutions (0.27 M, 1 M KOH) with different CuSO4
concentra-tions), the total amount of Cu2+ions was determined. For the hydrogel-microplate substrate, we obtained a total Cu2+-amount of 0.0038 mmol. Based on the ratio between the area of the blue region in Supplementary Fig. 7b and the printed squares of the paper background (0.634 × 0.634 cm2), the hydrogel area in the sample is estimated to be 1.30 cm2. Based on the estimated thickness of the con-tracted hydrogel of 10μm (Supplementary Fig. 1), the volume of the hydrogel is 0.00130 cm3. Therefore, the Cu2+concentration inside the contracted hydrogel is estimated to be 0.0038 mmol/0.00130 cm3= 2.9 M (Supplementary Fig. 7). The concentration of carboxylic acid groups in the hydrogel is estimated from the precursor solution, which was prepared from a solution of 0.4 mL acrylic acid + 0.5 mL ethylene glycol + 0.5 mL 1-butanol, and was subsequently mixed in a 9:1 ratio with the initiator solution, resulting in an acrylic acid concentration of 3.74 M. After the application of the hydrogel precursor, we assume that the solution wets the plates, with a height of 18μm, as well as the glass cover applied on top of it. Densiﬁcation of this precursor solution with a thickness of 18 μm to a hydrogel with aﬁnal thickness of 10 μm (see Supplementary Fig. 1) results in a ﬁnal car-boxylic acid concentration of 6.7 M. This indicates that after exposing to a con-centrated CuSO4solution, the Cu2+to COO−complexation in the hydrogel
approaches a 1:2 ratio (Cu2+/COO−max= 43%).
The data that support theﬁndings of this study are available within the article (and its Supplementary Informationﬁles) and from the corresponding authors on reasonable request.
The computer code that was developed to perform the simulations with our model is freely available at Github:https://github.com/nadirkaplan/hydrogels_naturecomm.
Received: 7 October 2019; Accepted: 12 December 2019;
1. Zhang, Y. S. & Khademhosseini, A. Advances in engineering hydrogels. Science 356, 500 (2017).
2. Ulijn, R. V. et al. Bioresponsive hydrogels. Mater. Today 10, 40–48 (2007). 3. Ionov, L. Hydrogel-based actuators: possibilities and limitations. Mater. Today
17, 494–503 (2014).
4. Schroeder, T. B. H. et al. An electric-eel-inspired soft power source from stacked hydrogels. Nature 552, 214–218 (2017).
5. Yuk, H. et al. Hydraulic hydrogel actuators and robots optically and sonically camouﬂaged in water. Nat. Commun. 8, 14230 (2017).
7. Shim, T. S., Kim, S.-H., Heo, C.-J., Jeon, H. C. & Yang, S.-M. Controlled origami folding of hydrogel bilayers with sustained reversibility for robust microcarriers. Angew. Chem. Int. Ed. 51, 1420–1423 (2012).
8. Kim, J., Hanna, J. A., Byun, M., Santangelo, C. D. & Hayward, R. C. Designing responsive buckled surfaces by halftone gel lithography. Science 335, 1201–1205 (2012).
9. Gladman, A. S., Matsumoto, E. A., Nuzzo, R. G., Mahadevan, L. & Lewis, J. A. Biomimetic 4D printing. Nat. Mater. 15, 413–418 (2016).
10. Ma, M., Guo, L., Anderson, D. G. & Langer, R. Bio-inspired polymer composite actuator and generator driven by water gradients. Science 339, 186–189 (2013).
11. Morales, D., Palleau, E., Dickey, M. D. & Velev, O. D. Electro-actuated hydrogel walkers with dual responsive legs. Soft Matter 10, 1337–1348 (2014). 12. Zhao, X. et al. Active scaffolds for on-demand drug and cell delivery. Proc.
Natl. Acad. Sci. USA 108, 67–72 (2011).
13. Zabow, G., Dodd, S. J. & Koretsky, A. P. Shape-changing magnetic assemblies as high-sensitivity NMR-readable nanoprobes. Nature 520, 73–77 (2015). 14. Dong, L., Agarwal, A. K., Beebe, D. J. & Jiang, H. Adaptive liquid microlenses
activated by stimuli-responsive hydrogels. Nature 442, 551–554 (2006). 15. He, X. et al. Synthetic homeostatic materials with chemo-mechano-chemical
self-regulation. Nature 487, 214–218 (2012).
16. Kim, Y. S. et al. Thermoresponsive actuation enabled by permittivity switching in an electrostatically anisotropic hydrogel. Nat. Mater. 14, 1002–1007 (2015). 17. Chin, S. M. et al. Covalent-supramolecular hybrid polymers as
muscle-inspired anisotropic actuators. Nat. Commun. 9, 2395 (2018).
18. Zhang, C., Cano, G. G. & Braun, P. V. Linear and fast hydrogel glucose sensor materials enabled by volume resetting agents. Adv. Mater. 26, 5678–5683 (2014). 19. Qin, M. et al. Bioinspired hydrogel interferometer for adaptive coloration and
chemical sensing. Adv. Mater. 30, 1800468 (2018).
20. Skoge, M. et al. Cellular memory in eukaryotic chemotaxis. Proc. Natl. Acad. Sci. USA 111, 14448–14453 (2014).
21. Nerbonne, J. M. & Kass, R. S. Molecular physiology of cardiac repolarization. Physiol. Rev. 85, 1205–1253 (2005).
22. Péter, M. et al. Metabolic crosstalk between membrane and storage lipids facilitates heat stress management in Schizosaccharomyces pombe. PLoS ONE 12, e0173739 (2017).
23. Bräutigam, K. et al. Dynamic plastid redox signals integrate gene expression and metabolism to induce distinct metabolic states in photosynthetic acclimation in Arabidopsis. Plant Cell 21, 2715–2732 (2009).
24. Kim, Y. S., Tamate, R., Akimoto, A. M. & Yoshida, R. Recent developments in self-oscillating polymeric systems as smart materials: from polymers to bulk hydrogels. Mater. Horiz. 4, 38–54 (2017).
25. Sidorenko, A., Krupenkin, T., Taylor, A., Fratzl, P. & Aizenberg, J. Reversible switching of hydrogel-actuated nanostructures into complex micropatterns. Science 315, 487–490 (2007).
26. Shastri, A. et al. An aptamer-functionalized chemomechanically modulated biomolecule catch-and-release system. Nat. Chem. 7, 447–454 (2015). 27. He, X., Friedlander, R. S., Zarzar, L. D. & Aizenberg, J. Chemo-mechanically
regulated oscillation of an enzymatic reaction. Chem. Mater. 25, 521–523 (2013). 28. Sidorenko, A., Krupenkin, T. & Aizenberg, J. Controlled switching of the
wetting behavior of biomimetic surfaces with hydrogel-supported nanostructures. J. Mater. Chem. 18, 3841–3846 (2008).
29. Liu, Y. et al. Computational modeling of oscillatingﬁns that “catch and release” targeted nanoparticles in bilayer ﬂows. Soft Matter 12, 1374–1384 (2016).
30. Palleau, E., Morales, D., Dickey, M. D. & Velev, O. D. Reversible patterning and actuation of hydrogels by electrically assisted ionoprinting. Nat. Commun. 4, 2257 (2013).
31. Grzybowski, B. A. & Huck, W. T. S. The nanotechology of life-inspired systems. Nat. Nanotechnol. 11, 585–592 (2016).
32. Dayal, P., Kuksenok, O. & Balazs, A. C. Reconﬁgurable assemblies of active, autochemotactic gels. Proc. Natl. Acad. Sci. USA 110, 431–436 (2013). 33. Cohen Stuart, M. A. et al. Emerging applications of stimuli-responsive
polymer materials. Nat. Mater. 9, 101–113 (2010).
34. Ashkenasy, G., Hermans, T. M., Otto, S. & Taylor, A. F. Systems chemistry. Chem. Soc. Rev. 46, 2543–2554 (2017).
35. Epstein, I. R. & Xu, B. Reaction-diffusion processes at the nano- and microscales. Nat. Nanotechnol. 11, 312–319 (2016).
36. Dhanarajan, A. P., Misra, G. P. & Siegel, R. A. Autonomous chemomechanical oscillations in a hydrogel/enzyme system driven by glucose. J. Phys. Chem. A 106, 8835–8838 (2002).
37. Wrobel, M. M. et al. pH Wave-front propagation in the urea-urease reaction. Biophys. J. 103, 610–615 (2012).
38. Cangialosi, A. et al. DNA sequence-directed shape change of photopatterned hydrogels via high-degree swelling. Science 357, 1126–1130 (2017). 39. Heinen, L., Heuser, T., Steinschulte, A. & Walther, A. Antagonistic enzymes in
a biocatalytic pH feedback system program autonomous DNA hydrogel life cycles. Nano Lett. 17, 4989–4995 (2017).
40. Fets, L., Kay, R. & Velazquez, F. Dictyostelium. Curr. Biol. 20, R1008 (2010). 41. Mahadevan, L. & Matsudaira, P. Motility powered by supramolecular springs
and ratchets. Science 288, 95–99 (2000).
42. Hu, Y., Kim, P. & Aizenberg, J. Harnessing structural instability and material instability in the hydrogel-actuated integrated responsive structures (HAIRS). Extrem. Mech. Lett. 13, 84–90 (2017).
This material is based upon work supported by the Department of Energy under Award Number DE-SC0005247. P.A.K. thanks the Netherlands Organisation for Scientiﬁc Research (NWO Rubicon, VENI) and the Ministry of Education, Culture and Science (Gravity program, 024.001.035) forﬁnancial support. We thank M. Aizenberg, L. Mahadevan and T. Schroeder for stimulating discussions.
P.A.K., A.G. and J.A. conceived the research. P.A.K. and R.M.R. performed the experi-ments; C.N.K. developed the theoretical model; all authors analyzed the results; P.A.K., C.N.K., A.G. and J.A. wrote the manuscript.
The authors declare no competing interests.
Supplementary informationis available for this paper at https://doi.org/10.1038/s41467-019-14114-0.
Correspondenceand requests for materials should be addressed to P.A.K., C.N.K. or J.A.
Peer review informationNature Communications thanks the anonymous reviewer(s) for their contribution to the peer review of this work.
Reprints and permission informationis available athttp://www.nature.com/reprints
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations.
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visithttp://creativecommons.org/ licenses/by/4.0/.